# UNS C47000 (RBCuZn-A) Filler Metal

C47000 brass is a copper-based filler metal for brazing. Cited properties are appropriate for the as-fabricated (no temper or treatment) condition. RBCuZn-A is the AWS designation for this material. C47000 is the UNS number.

It has the highest ductility among the copper-based braze fillers in the database.

The graph bars on the material properties cards below compare C47000 brass to: copper-based braze fillers (top), all copper alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Elastic (Young's, Tensile) Modulus

100 *GPa* 15 *x 10 ^{6} psi*

Elongation at Break

36 *%*

Poisson's Ratio

0.3

Shear Modulus

40 *GPa* 5.8 *x 10 ^{6} psi*

Tensile Strength: Ultimate (UTS)

380 *MPa* 55 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

150 *MPa* 21 *x 10 ^{3} psi*

## Thermal Properties

Brazing Temperature

910 to 950 *°C* 1670 to 1750 *°F*

Latent Heat of Fusion

170 *J/g*

Maximum Temperature: Mechanical

120 *°C* 240 *°F*

Melting Completion (Liquidus)

900 *°C* 1650 *°F*

Melting Onset (Solidus)

890 *°C* 1630 *°F*

Specific Heat Capacity

390 *J/kg-K* 0.092 *BTU/lb-°F*

Thermal Conductivity

120 *W/m-K* 67 *BTU/h-ft-°F*

Thermal Expansion

21 *µm/m-K*

## Otherwise Unclassified Properties

Base Metal Price

23 *% relative*

Density

8.0 *g/cm ^{3}* 500

*lb/ft*

^{3}Embodied Carbon

2.7 *kg CO _{2}/kg material*

Embodied Energy

47 *MJ/kg* 20 *x 10 ^{3} BTU/lb*

Embodied Water

330 *L/kg* 39 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

110 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

100 *kJ/m ^{3}*

Stiffness to Weight: Axial

7.2 *points*

Stiffness to Weight: Bending

20 *points*

Strength to Weight: Axial

13 *points*

Strength to Weight: Bending

15 *points*

Thermal Diffusivity

38 *mm ^{2}/s*

Thermal Shock Resistance

13 *points*

## Alloy Composition

Cu | 57 to 61 | |

Zn | 37.5 to 42.8 | |

Sn | 0.25 to 1.0 | |

Pb | 0 to 0.050 | |

Al | 0 to 0.010 | |

res. | 0 to 0.4 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Similar Alloys

## Further Reading

AWS A5.8: Specification for Filler Metals for Brazing and Braze Welding